Submitted to Journal of Materials Research & Technology (February 2016)
Achieving superplastic properties in a ZK10 magnesium alloy
processed by equal-channel angular pressing
Roberto B. Figueiredo1,*, Terence G. Langdon2,3
1 Department of Materials Engineering and Civil Construction, Universidade Federal
de Minas Gerais, Belo Horizonte, MG 31270-901, Brazil
2 Materials Research Group, Faculty of Engineering and the Environment, University
of Southampton, Southampton SO17 1BJ, U.K.
3 Departments of Aerospace & Mechanical Engineering and Materials Science,
University of Southern California, Los Angeles, CA 90089-1453, U.S.A.
Abstract: Equal-channel angular pressing provides an opportunity for refining the
grain structure and introducing superplastic properties in magnesium alloys. This
report describes the use of this processing technique with a ZK10 (Mg-1.0 wt.% Zn-
0.26 wt.% Zr) alloy. The grain structure was successfully refined from ~12.9 to ~5.2
µm after 4 passes and superplastic elongations were observed when testing at low
strain rates at temperatures of 473 and 523 K. An analysis shows that the
superplastic behavior is consistent with the conventional theoretical model for
superplastic flow and at higher stresses and strain rates there is a transition to
control by a viscous glide process.
Keywords: equal-channel angular pressing; magnesium alloy; superplasticity;
viscous glide; ZK10.
*corresponding author: email@example.com (+55) 31 3409-1751
Magnesium and its alloys usually exhibit low ductility at low temperatures and
this is due to the limited number of active slip systems that are available to
accommodate the plastic deformation. It is well established that an increasing
temperature leads to the activation of additional slip systems thereby improving the
formability of these materials . Furthermore, provided the grain structure is
sufficiently fine, with average grain sizes smaller than ~10 µm, a significant portion of
the plastic deformation may arise from grain boundary sliding (GBS) at high
temperatures . The occurrence of GBS is linked to a high value of the strain rate
sensitivity which inhibits strain localization and permits the material to pull out in
tension to very large superplastic elongations without failure. This superplastic flow
is important in industrial applications because it provides an opportunity to produce
complex curved shapes through simple forming operations .
Superplasticity is a diffusion-controlled process requiring both a fine grain size
and a high testing temperature, typically above ~0.5Tm where Tm is the absolute
melting temperature. At these high temperatures, a fine grain size is most easily
retained through the presence of second phase precipitates and in magnesium
alloys superplasticity has been reported in alloys containing precipitates such as
AZ61 [4,5] and ZK60 . Also, the material must be processed in order to obtain a
fine-grained structure and this is generally undertaken using powder metallurgy
techniques . More recently, the development of processing procedures based on
the application of severe plastic deformation (SPD) has provided opportunities for
achieving exceptional grain refinement in many metallic alloys, including magnesium
alloys, together with significant superplastic properties .
Although there are several different SPD processing methods, most attention
to date has focused on equal-channel angular pressing (ECAP) where a rod or bar is
pressed through a die constrained within a channel  or high-pressure torsion
(HPT) where a thin disk is subjected to compression and concurrent torsional
straining . Comprehensive reviews are now available documenting the
experimental data reported for superplasticity in alloys processed using ECAP and
HPT [11-13]. Initially, significant attention was given to the ZK60 alloy (Mg- 5.5 wt.%
Zn-0.5 wt.% Zr) which exhibits excellent superplastic properties after processing by
ECAP [14-21] including a potential for attaining high strain rate superplasticity 
and the development of a record superplastic elongation of more than 3000% .
In addition to the excellent superplastic properties recorded in the ZK60 alloy, other
magnesium alloys also exhibit superplasticity after processing by ECAP including the
single phase AZ31 alloy [22-26]. However, despite the excellent superplastic
properties introduced in a single phase magnesium alloy having aluminum in solid
solution, there has been only limited research to date to evaluate the potential for
achieving superplasticity in other dilute magnesium alloys. For example, it was
reported recently that ECAP processing leads to low temperature superplasticity in a
ZM21 (Mg-1.78 wt.% Zn-0.89 wt.% Mn) alloy .
Accordingly, the present research was initiated to evaluate the potential for
achieving superplastic ductilities in a more dilute ZK10 alloy (Mg-1.0 wt.% Zn-0.25
wt.% Zr). This alloy was selected because excellent superplastic properties were
already reported in the ZK60 magnesium alloy which has a much higher zinc content
and both ZK60 and ZK10 have zinc and zirconium as the major alloying elements.
As will be demonstrated, superplastic properties are also attained in the ZK10 alloy
but the elongations are significantly lower than in the ZK60 alloy.
2. Experimental material and procedures
The experiments were conducted using a magnesium ZK10 alloy supplied by
Magnesium Elektron (Riverside, CA) as rolled slabs. The composition of the alloy is
shown in Table 1. Billets with diameters of 10 mm and lengths of 60 mm were
machined from the slabs with the axial directions parallel to the rolling direction.
These billets were processed by ECAP at a temperature of 493 K using a die with an
angle of 110° between the two channels and with an outer arc of curvature of 20° at
the intersection of the two channels. These angles in the ECAP die produce a strain
of ~0.8 on each separate pass through the die  and the billets were processed for
up to 4 passes using route Bc in which the billet is rotated by 90° in the same sense
between each pass .
Samples of the material were extracted before and after ECAP processing for
metallography. The samples were ground on silica carbide papers and polished to a
mirror-like finish on cloth using alumina oxide and ethanol as abrasive media. The
grain boundaries were revealed by etching with acetic-picral (70 mL of ethanol, 4.2 g
of picric acid, 10 mL of acetic acid and 10 mL of water). The average grain size was
determined as d = 1.74 × L where L is the mean intercept length.
Tensile specimens with gauge lengths of 4 mm and cross-sections of 2 × 3
mm2 were machined from the processed billets and tested in tension at different
temperatures and strain rates. Load and displacement data were converted to true
stress-true strain curves by assuming volume constancy and homogeneous
deformation. The machine elastic distortion was corrected by equating the elastic
region of the curve to the theoretical elastic modulus of the material.
3. Experimental results
3.1 Grain structure after ECAP
Figure 1 shows representative images of the grain structures of the material
before and after processing by ECAP. It was observed that etching does not reveal
all of the grain boundaries with the same intensity. Thus, some boundaries are
readily visible and others are poorly defined. The average grain size in the as
received condition in Fig. 1(a) was measured as ~12.9 µm. Processing by ECAP
promoted significant grain refinement. After only 2 passes in Fig. 2(b) the structure
became bimodal with some larger grains and areas of smaller grains of a few
micrometers. This bimodal grain size distribution is generally expected in
magnesium alloys due to the mechanism of grain refinement in which new fine
grains are formed preferentially along the grain boundaries while the cores of the
original grains remain unrefined [30,31]. After 2 passes the average grain size was
~6.8 µm. Similar features were also observed in the alloy after 4 passes of ECAP as
shown in Fig. 1(c) where the average grain size was slightly smaller at d ≈ 5.2 µm.
3.2 Tensile testing
Tensile tests were carried out at different temperatures in the range from 473
to 573 K after processing through 4 passes of ECAP. Figure 2 shows the recorded
elongations when testing with an initial strain rate of 1.0 × 10-4 s-1 plotted as a
function of the testing temperature, T. Thus, high elongations of ~500% are
observed at 473 and 493 K and there is a peak elongation of 750% at 523 K.
Thereafter, there is a sharp reduction in elongation to
there is a capability for achieving superplastic flow in the ZK10 alloy at temperatures
up to ~540 K.
Tensile tests were also carried out on samples of the material processed by
only 2 passes of ECAP and Fig. 3(a) shows plots of true stress and true strain for
tests conducted at temperatures of 473 and 523 K for tests at an initial strain rate of
1.0 × 10-3 s-1. Also shown in Fig. 3(a) are curves for samples tested under these
conditions after 4 passes of ECAP. Inspection shows processing through 4 passes
leads to lower flow stresses at both temperatures. This difference in flow stress is
due to the finer grain size achieved in the material after processing through 4
Similar stress-strain curves are shown in Fig. 3(b) for tests conducted on the
material processed for 4 passes of ECAP at different initial strain rates from 10-4 to
10-2 s-1 and at the two temperatures of 473 and 523 K. It is readily ob